#------------------------------------------------------------------------------
#$Date: 2016-03-26 20:42:49 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180445 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/14/7211446.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7211446
loop_
_publ_author_name
'Yang, Bing-Ping'
'Xu, Xiang'
'Huang, Chao'
'Mao, Jiang-Gao'
_publ_section_title
;
 K4TM4(V2O7)2(IO3)4(H2O) (TM = Zn, Ni, Co): a series of quinary mixed
 metal--vanadium(v)--iodates
;
_journal_issue                   48
_journal_name_full               CrystEngComm
_journal_page_first              10464
_journal_paper_doi               10.1039/c3ce41653d
_journal_volume                  15
_journal_year                    2013
_chemical_formula_moiety         '2(Co2 I2 O13 V2), 2(O0.50)2H, 4.0(K) '
_chemical_formula_sum            'Co4 H2 I4 K4 O27 V4'
_chemical_formula_weight         1537.50
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   5.5840(2)
_cell_length_b                   5.5840(2)
_cell_length_c                   25.991(2)
_cell_measurement_reflns_used    2659
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4680
_cell_measurement_theta_min      2.1056
_cell_volume                     701.85(6)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2007)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0288
_diffrn_reflns_av_sigmaI/netI    0.0124
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       33
_diffrn_reflns_limit_l_min       -33
_diffrn_reflns_number            5363
_diffrn_reflns_theta_full        27.47
_diffrn_reflns_theta_max         27.47
_diffrn_reflns_theta_min         4.21
_exptl_absorpt_coefficient_mu    8.668
_exptl_absorpt_correction_T_max  0.841
_exptl_absorpt_correction_T_min  0.093
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   Higashi
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    3.638
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Plate
_exptl_crystal_F_000             706
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.3
_exptl_crystal_size_min          0.02
_refine_diff_density_max         1.231
_refine_diff_density_min         -1.181
_refine_diff_density_rms         0.180
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.212
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     38
_refine_ls_number_reflns         553
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.212
_refine_ls_R_factor_all          0.0279
_refine_ls_R_factor_gt           0.0270
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0342P)²+2.2016P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0689
_refine_ls_wR_factor_ref         0.0697
_reflns_number_gt                534
_reflns_number_total             553
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3ce41653d.cif
_cod_data_source_block           K4Co4(V2O7)2(IO3)4(H2O)
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_H-M      P6(3)/m
_cod_database_code               7211446
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
K1 K 0.3333 0.6667 0.2500 0.0320(12) Uani 0.657(10) 6 d SP
K2 K 0.3333 0.6667 -0.01940(13) 0.0570(11) Uani 0.672(5) 3 d SP
Co1 Co 0.3333 0.6667 0.11612(4) 0.0161(2) Uani 1 3 d S
V1 V -0.3333 0.3333 0.18154(4) 0.0100(2) Uani 1 3 d S
I1 I 0.0000 0.0000 0.102031(15) 0.01317(18) Uani 1 3 d S
O1 O 0.1080(5) 0.3219(5) 0.06841(11) 0.0209(6) Uani 1 1 d .
O2 O -0.3333 0.3333 0.2500 0.049(3) Uani 1 6 d S
O3 O -0.0165(6) 0.5651(6) 0.15999(12) 0.0253(6) Uani 1 1 d .
O1W O 0.0000 1.0000 0.2500 0.027(3) Uani 0.50 6 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 K1 O3 145.27(5) 12_566 .
O3 K1 O3 62.26(9) 12_566 10_556
O3 K1 O3 106.69(11) . 10_556
O3 K1 O3 62.26(9) 12_566 11_666
O3 K1 O3 145.27(5) . 11_666
O3 K1 O3 62.26(9) 10_556 11_666
O3 K1 O3 106.69(12) 12_566 3_565
O3 K1 O3 62.26(9) . 3_565
O3 K1 O3 145.27(5) 10_556 3_565
O3 K1 O3 145.27(5) 11_666 3_565
O3 K1 O3 145.27(5) 12_566 2_665
O3 K1 O3 62.26(9) . 2_665
O3 K1 O3 145.27(5) 10_556 2_665
O3 K1 O3 106.69(11) 11_666 2_665
O3 K1 O3 62.26(9) 3_565 2_665
O3 K1 O2 114.32(7) 12_566 .
O3 K1 O2 54.53(6) . .
O3 K1 O2 54.53(5) 10_556 .
O3 K1 O2 99.70(6) 11_666 .
O3 K1 O2 114.32(7) 3_565 .
O3 K1 O2 99.70(6) 2_665 .
O3 K1 O2 54.53(5) 12_566 1_665
O3 K1 O2 99.70(6) . 1_665
O3 K1 O2 99.70(6) 10_556 1_665
O3 K1 O2 114.32(7) 11_666 1_665
O3 K1 O2 54.53(5) 3_565 1_665
O3 K1 O2 114.32(7) 2_665 1_665
O2 K1 O2 120.0 . 1_665
O3 K1 O1W 80.30(6) 12_566 .
O3 K1 O1W 65.68(7) . .
O3 K1 O1W 65.68(7) 10_556 .
O3 K1 O1W 125.47(5) 11_666 .
O3 K1 O1W 80.30(6) 3_565 .
O3 K1 O1W 125.47(5) 2_665 .
O2 K1 O1W 60.0 . .
O2 K1 O1W 60.0 1_665 .
O3 K1 O1W 65.68(7) 12_566 1_655
O3 K1 O1W 125.47(6) . 1_655
O3 K1 O1W 125.47(6) 10_556 1_655
O3 K1 O1W 80.30(6) 11_666 1_655
O3 K1 O1W 65.68(7) 3_565 1_655
O3 K1 O1W 80.30(6) 2_665 1_655
O2 K1 O1W 180.0 . 1_655
O2 K1 O1W 60.0 1_665 1_655
O1W K1 O1W 120.0 . 1_655
O3 K1 O1W 125.47(5) 12_566 1_545
O3 K1 O1W 80.30(6) . 1_545
O3 K1 O1W 80.30(6) 10_556 1_545
O3 K1 O1W 65.68(7) 11_666 1_545
O3 K1 O1W 125.47(5) 3_565 1_545
O3 K1 O1W 65.68(7) 2_665 1_545
O2 K1 O1W 60.0 . 1_545
O2 K1 O1W 180.0 1_665 1_545
O1W K1 O1W 120.0 . 1_545
O1W K1 O1W 120.0 1_655 1_545
O3 K1 O2 99.70(6) 12_566 1_655
O3 K1 O2 114.32(7) . 1_655
O3 K1 O2 114.32(7) 10_556 1_655
O3 K1 O2 54.53(5) 11_666 1_655
O3 K1 O2 99.70(6) 3_565 1_655
O3 K1 O2 54.53(5) 2_665 1_655
O2 K1 O2 120.0 . 1_655
O2 K1 O2 120.0 1_665 1_655
O1W K1 O2 180.0 . 1_655
O1W K1 O2 60.0 1_655 1_655
O1W K1 O2 60.0 1_545 1_655
O1 K2 O1 100.97(11) 7_565 9_665
O1 K2 O1 100.97(11) 7_565 8
O1 K2 O1 100.97(11) 9_665 8
O1 K2 O1 87.20(11) 7_565 3_565
O1 K2 O1 106.49(8) 9_665 3_565
O1 K2 O1 149.29(11) 8 3_565
O1 K2 O1 149.29(11) 7_565 2_665
O1 K2 O1 87.20(11) 9_665 2_665
O1 K2 O1 106.49(8) 8 2_665
O1 K2 O1 62.14(11) 3_565 2_665
O1 K2 O1 106.49(8) 7_565 .
O1 K2 O1 149.29(11) 9_665 .
O1 K2 O1 87.20(11) 8 .
O1 K2 O1 62.14(11) 3_565 .
O1 K2 O1 62.14(11) 2_665 .
O1 K2 O1 56.22(10) 7_565 9
O1 K2 O1 130.51(15) 9_665 9
O1 K2 O1 52.17(10) 8 9
O1 K2 O1 114.34(7) 3_565 9
O1 K2 O1 136.17(9) 2_665 9
O1 K2 O1 77.59(10) . 9
O1 K2 O1 52.17(10) 7_565 8_565
O1 K2 O1 56.22(10) 9_665 8_565
O1 K2 O1 130.51(15) 8 8_565
O1 K2 O1 77.59(10) 3_565 8_565
O1 K2 O1 114.34(7) 2_665 8_565
O1 K2 O1 136.17(9) . 8_565
O1 K2 O1 106.37(8) 9 8_565
O1 K2 O1 130.51(15) 7_565 7_665
O1 K2 O1 52.17(10) 9_665 7_665
O1 K2 O1 56.22(10) 8 7_665
O1 K2 O1 136.17(9) 3_565 7_665
O1 K2 O1 77.59(10) 2_665 7_665
O1 K2 O1 114.34(7) . 7_665
O1 K2 O1 106.37(8) 9 7_665
O1 K2 O1 106.37(8) 8_565 7_665
O1 K2 K2 96.71(6) 7_565 7_675
O1 K2 K2 53.77(7) 9_665 7_675
O1 K2 K2 151.79(8) 8 7_675
O1 K2 K2 52.72(9) 3_565 7_675
O1 K2 K2 64.29(10) 2_665 7_675
O1 K2 K2 108.68(16) . 7_675
O1 K2 K2 152.34(5) 9 7_675
O1 K2 K2 50.04(6) 8_565 7_675
O1 K2 K2 95.62(5) 7_665 7_675
O1 K2 K2 53.77(7) 7_565 7_565
O1 K2 K2 151.79(8) 9_665 7_565
O1 K2 K2 96.71(6) 8 7_565
O1 K2 K2 64.29(10) 3_565 7_565
O1 K2 K2 108.68(16) 2_665 7_565
O1 K2 K2 52.72(9) . 7_565
O1 K2 K2 50.04(6) 9 7_565
O1 K2 K2 95.62(5) 8_565 7_565
O1 K2 K2 152.34(5) 7_665 7_565
K2 K2 K2 111.49(10) 7_675 7_565
O1 K2 K2 151.79(8) 7_565 7_665
O1 K2 K2 96.71(6) 9_665 7_665
O1 K2 K2 53.77(7) 8 7_665
O1 K2 K2 108.68(16) 3_565 7_665
O1 K2 K2 52.72(9) 2_665 7_665
O1 K2 K2 64.29(10) . 7_665
O1 K2 K2 95.62(5) 9 7_665
O1 K2 K2 152.34(5) 8_565 7_665
O1 K2 K2 50.04(6) 7_665 7_665
K2 K2 K2 111.49(10) 7_675 7_665
K2 K2 K2 111.49(10) 7_565 7_665
O3 Co1 O3 92.85(12) 3_565 .
O3 Co1 O3 92.85(12) 3_565 2_665
O3 Co1 O3 92.85(12) . 2_665
O3 Co1 O1 175.82(12) 3_565 .
O3 Co1 O1 91.33(11) . .
O3 Co1 O1 87.17(11) 2_665 .
O3 Co1 O1 91.33(11) 3_565 3_565
O3 Co1 O1 87.17(11) . 3_565
O3 Co1 O1 175.82(12) 2_665 3_565
O1 Co1 O1 88.65(11) . 3_565
O3 Co1 O1 87.17(11) 3_565 2_665
O3 Co1 O1 175.82(12) . 2_665
O3 Co1 O1 91.33(11) 2_665 2_665
O1 Co1 O1 88.65(11) . 2_665
O1 Co1 O1 88.65(11) 3_565 2_665
O3 Co1 K1 56.78(9) 3_565 .
O3 Co1 K1 56.78(9) . .
O3 Co1 K1 56.78(9) 2_665 .
O1 Co1 K1 126.22(8) . .
O1 Co1 K1 126.22(8) 3_565 .
O1 Co1 K1 126.22(8) 2_665 .
O3 Co1 K2 123.22(9) 3_565 .
O3 Co1 K2 123.22(9) . .
O3 Co1 K2 123.22(9) 2_665 .
O1 Co1 K2 53.78(8) . .
O1 Co1 K2 53.78(8) 3_565 .
O1 Co1 K2 53.78(8) 2_665 .
K1 Co1 K2 180.0 . .
O3 V1 O3 109.49(11) 3_455 .
O3 V1 O3 109.49(11) 3_455 2_565
O3 V1 O3 109.49(11) . 2_565
O3 V1 O2 109.46(11) 3_455 .
O3 V1 O2 109.46(11) . .
O3 V1 O2 109.46(11) 2_565 .
O3 V1 K1 112.02(12) 3_455 .
O3 V1 K1 50.47(10) . .
O3 V1 K1 138.11(11) 2_565 .
O2 V1 K1 61.106(14) . .
O3 V1 K1 50.47(10) 3_455 1_445
O3 V1 K1 138.11(11) . 1_445
O3 V1 K1 112.02(12) 2_565 1_445
O2 V1 K1 61.106(14) . 1_445
K1 V1 K1 98.614(18) . 1_445
O3 V1 K1 138.11(11) 3_455 1_455
O3 V1 K1 112.02(12) . 1_455
O3 V1 K1 50.47(10) 2_565 1_455
O2 V1 K1 61.106(14) . 1_455
K1 V1 K1 98.614(18) . 1_455
K1 V1 K1 98.614(18) 1_445 1_455
O1 I1 O1 98.63(12) 2 .
O1 I1 O1 98.63(12) 2 3
O1 I1 O1 98.63(12) . 3
O1 I1 K2 41.97(9) 2 7
O1 I1 K2 116.63(10) . 7
O1 I1 K2 59.47(9) 3 7
O1 I1 K2 59.47(9) 2 7_565
O1 I1 K2 41.97(8) . 7_565
O1 I1 K2 116.63(10) 3 7_565
K2 I1 K2 92.23(6) 7 7_565
O1 I1 K2 116.63(10) 2 7_665
O1 I1 K2 59.47(9) . 7_665
O1 I1 K2 41.97(9) 3 7_665
K2 I1 K2 92.23(6) 7 7_665
K2 I1 K2 92.23(6) 7_565 7_665
I1 O1 Co1 112.03(14) . .
I1 O1 K2 112.45(12) . 7_565
Co1 O1 K2 112.22(11) . 7_565
I1 O1 K2 151.12(15) . .
Co1 O1 K2 89.64(10) . .
K2 O1 K2 73.51(8) 7_565 .
I1 O1 K2 92.72(10) . 7_665
Co1 O1 K2 94.70(10) . 7_665
K2 O1 K2 130.51(15) 7_565 7_665
K2 O1 K2 65.66(7) . 7_665
V1 O2 V1 180.0 10_556 .
V1 O2 K1 90.0 10_556 .
V1 O2 K1 90.0 . .
V1 O2 K1 90.0 10_556 1_445
V1 O2 K1 90.0 . 1_445
K1 O2 K1 120.0 . 1_445
V1 O2 K1 90.0 10_556 1_455
V1 O2 K1 90.0 . 1_455
K1 O2 K1 120.0 . 1_455
K1 O2 K1 120.0 1_445 1_455
V1 O3 Co1 151.1(2) . .
V1 O3 K1 103.12(13) . .
Co1 O3 K1 86.57(10) . .
K1 O1W K1 120.0 . 1_565
K1 O1W K1 120.0 . 1_455
K1 O1W K1 120.0 1_565 1_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
K1 O3 2.916(3) 12_566
K1 O3 2.916(3) .
K1 O3 2.916(3) 10_556
K1 O3 2.916(3) 11_666
K1 O3 2.916(3) 3_565
K1 O3 2.916(3) 2_665
K1 O2 3.22392(11) .
K1 O2 3.22392(11) 1_665
K1 O1W 3.22392(11) .
K1 O1W 3.22392(11) 1_655
K1 O1W 3.22392(12) 1_545
K1 O2 3.22392(11) 1_655
K2 O1 2.803(3) 7_565
K2 O1 2.803(3) 9_665
K2 O1 2.803(3) 8
K2 O1 2.842(4) 3_565
K2 O1 2.842(4) 2_665
K2 O1 2.842(4) .
K2 O1 3.340(3) 9
K2 O1 3.340(3) 8_565
K2 O1 3.340(3) 7_665
K2 K2 3.378(2) 7_675
K2 K2 3.378(2) 7_565
K2 K2 3.378(2) 7_665
Co1 O3 2.081(3) 3_565
Co1 O3 2.081(3) .
Co1 O3 2.081(3) 2_665
Co1 O1 2.099(3) .
Co1 O1 2.099(3) 3_565
Co1 O1 2.099(3) 2_665
V1 O3 1.682(3) 3_455
V1 O3 1.682(3) .
V1 O3 1.682(3) 2_565
V1 O2 1.7793(10) .
V1 K1 3.6823(5) 1_445
V1 K1 3.6823(5) 1_455
I1 O1 1.809(3) 2
I1 O1 1.809(3) .
I1 O1 1.809(3) 3
I1 K2 3.8738(19) 7
I1 K2 3.8738(19) 7_565
I1 K2 3.8738(19) 7_665
O1 K2 2.803(3) 7_565
O1 K2 3.340(3) 7_665
O2 V1 1.7793(10) 10_556
O2 K1 3.22392(12) 1_445
O2 K1 3.22392(11) 1_455
O1W K1 3.22392(11) 1_565
O1W K1 3.22392(11) 1_455
